The crystal structure of bulk SrTiO3(STO) transitions from cubic to tetragonal at around 105 K. Recent local scanning probe measurements of LaAlO3/SrTiO3 (LAO/STO) interfaces indicated the existence of spatially inhomogeneous electrical current paths and electrostatic potential associated with the structural domain formation in the tetragonal phase of STO. Here we report a study of temperature dependent electronic transport in combination with the polarized light microscopy of structural domains in mesoscopic LAO/STO devices. By reducing the size of the conductive interface to be comparable to that of a single tetragonal domain of STO, the anisotropy of interfacial electron conduction in relationship to the domain wall and its direction was characterized between T = 10–300 K. It was found that the four-point resistance measured with current parallel to the domain wall is larger than the resistance measured perpendicular to the domain wall. This observation is qualitatively consistent with the current diverting effect from a more conductive domain wall within the sample. Among all the samples studied, the maximum resistance ratio found is at least 10 and could be as large as 105 at T = 10 K. This electronic anisotropy may have implications on other oxide hetero-interfaces and the further understanding of electronic/magnetic phenomena found in LAO/STO.
The structures and structural phase transitions of SrTiO3 had been a subject of research interests since decades ago1,2. Since the discovery of quasi-two-dimensional(q2D) electron conduction between LaAlO3 and TiO2 terminated SrTiO3 in 20043, LAO/STO heterointerfaces have quickly become one of the fastest growing research fields in physics and material science research4,5,6,7. While LAO/STO is being explored for novel nanoelectronic and memory device applications8,9,10,11, researchers also uncovered many exotic phenomena in LAO/STO such as gate tunable conductivity and superconductivity12,13,14, magnetism15 and even the coexistence of magnetism with superconductivity16,17,18,19. Thanks to the success of LAO/STO, oxide based heterostructures are experiencing a significant boom in research focus20. Al2O3/SrTiO321,22, LaCoO3/SrTiO323, GdTiO3/SrTiO324, and SmTiO3/SrTiO325 are just a few of the many exciting materials that have been realized due to this concentration in oxide heterointerfaces.
Along with numerous physical phenomena, perovskite oxide heterointerface systems boast complexities that rival high-Tc superconductors. Oxygen growth pressure26,27,28, La/Al stoichometry29, and cation intermixing30,31 are a few of known factors that can affect interfacial conduction in LAO/STO. Recently, scanning probe or scanning electron microscopy techniques showed that crystal domain boundaries in the STO layer of LAO/STO modify the local conductivity of the interface and create regions of striped potential modulations32,33,34. However, it is unclear if such microscopic effects would impact the electrical devices based on LAO/STO in any gross way. In an electrical transport study of macroscopic LAO/STO samples with size about 5 mm × 5 mm, Schoofs et al.35 discovered hysteresis effects between the warm up and cool down temperature (T) dependent resistance R(T) at T ~ 85 K as well as ~180 K in samples with q2D electron density a few times 1013/cm2 and the q2D confinement is strong. These hysteresis effects were attributed to structural phase transitions whose transition temperature may be different from the bulk due to the surface nature of the LAO/STO. But the exact nature of these two structural transitions were not known. In the present work, we combined the polarized light microscopy imaging of structural domains and direct electrical transport measurement of the same device for the first time and obtained two new findings. First, we identified the hysteretic R(T) ~ 85 K in LAO/STO to be related to the cubic to tetragonal transition as confirmed by in situ polarized light microscopy. The higher temperature hysteresis/transition at ~180 K does not induce any feature detectable by polarized microscopy. Moreover, we found that mesoscopic LAO/STO devices containing single tetragonal domain walls exhibit anisotropic electron transport at low temperatures: the resistance ratio between the current parallel to the domain wall versus current perpendicular to the domain wall configurations is at least ten at 10 K and could reach as high as 105 in a sample which showed diverging insulating R(T) at low T along the high resistance configuration. In addition to the potential relevance to the understanding of other non-uniform properties of oxide hetero-interfaces, this striking resistance anisotropy in mesoscopic LAO/STO samples with domain walls should be considered in the future study of oxide electronics and may be exploited for applications.
In this study, characterization of LAO/STO is performed on samples grown by pulsed laser deposition (PLD). Most of samples studied had 10 unit cell (10 u.c.) LAO and were deposited at O2 partial pressure of 10−4 or 10−5 Torr, although an 8 u.c. sample was also studied for comparison. Fig. 1a shows a typical scanning transmission electron microscopy (STEM) image recorded on a LAO/STO sample with 10 u.c. LAO film. Although a small level of cation intermixing is likely to have occurred31, the PLD growth resulted in well-defined interfaces with no misfit dislocation detected (Fig. 1a and Supplementary Figure S1). The samples were found to have electron density in the range of 1013–1015/cm2 at room temperature, consistent with literature for LAO thicknesses above the critical thickness of 4 u.c.
It has been known since the 1960’s that SrTiO3 exhibits a cubic to a non-polar tetragonal phase transition at critical temperature Tc ~ 105 K, driven by the rotation of TiO6 octahedron along the elongated c-axis, as it is cooled from room temperature1,2,32,33,34. Using polarized light microscopy, the tetragonal crystal domains in the STO substrate of LAO/STO can be imaged and characterized2,32. A continuous flow microscopy cryostat with an optical window allowed us to image tetragonal domains and domain wall formation in the LAO/STO samples and correlate domain formation with in situ transport measurements. Figure 1b shows the disappearance of tetragonal domains over a representative area upon warming up a 5 mm × 5 mm sized 10 u.c. sample between 77 K–100 K. In these images, striped tetragonal domains are 20–40 μm wide, consistent with previously published results2,32,33. In such domain imaging experiments, striped tetragonal domains typically start to show visible disappearance around 90 K and appear to be completely disappeared around 100 K (Fig. 1b), close to the ~85 K R(T) hysteresis seen in ref. 35 and the frequently cited Tc ~ 105 K in bulk STO. Accompanying the disappearance of tetragonal domains between 90 K–100 K is a hysteresis effect observed in the temperature dependent resistance, R(T). Cool-down and warm-up resistance curves show some deviation below 90 K (Fig. 1c). We observe that while the cool-down R(T) is always smooth across the cubic-tetragonal transition of STO, R(T) during warm-up often shows a kink when the tetragonal domains start to disappear as shown in Fig. 1c. In our study here where the R(T) hysteresis around 90 K is more pronounced than ref. 35, simultaneous resistance and polarized imaging measurements reveal that such hysteresis R(T) is associated with the tetragonal domain formation/disappearance and domains are not detected above 100 K in polarized light microscopy similar to ref. 32,33. We also note that in our experiments, thermally cycling the sample across the transition temperature appears to induce very little change to the domain pattern (Supplementary Figure S2), although the thermal cycling process sometimes causes the imaging focus to be slightly off the surface and artificially causes the domain pattern to change. The consistent domain pattern upon thermal cycling suggests that instead of being random, the domain nucleation process is likely dominated by fixed crystalline defects in our samples. This ‘memory’ effect of domain walls originated from inherent defects in the STO was also seen in a recent paper (ref. 34) although in ref. 34, many finer domain patterns were found to change upon thermal cycling to room T.
Under the cubic-to-tetragonal transition temperature, twin domains averaging about 30 μm wide run parallel or perpendicular to each other and are split by domain walls, as shown in Fig. 1. Thus when electron transport in a macroscopic sample is measured, any unique carrier transport effects due to individual domains and domain boundaries (e.g. local conductivity modulation32 or anisotropy) could be averaged out, explaining the generally small magnitude of the hysteresis seen in transport data around Tc on large samples (Fig. 1 and ref. 35). To clearly understand the intrinsic electrical transport due to domains and domain walls in LAO/STO device, the measurement area was reduced to the order of the domain size. Photolithography and wet etching techniques were performed on LAO/STO to reduce the spatial size of the conductive interface to 10 × 10 μm2–40 × 40 μm2 van der Pauw squares (Fig. 2c,d). Figure 2 (a) and (b) compare the temperature dependent resistance normalized over the 300 K resistance value R0, for a 10 u.c. sample before (a) and after (b) reducing the conductive area from 5 × 5 mm2 to 40 × 40 μm2 (unless noted, R(T) curves shown were taken during the cool-down). R1 and R2 are the four-wire resistances measured with current flow directions at 90° to each other. Before micro-patterning, R1 and R2 showed consistent temperature dependence throughout the whole temperature range covered (10–300 K) (Fig. 2a). Note that although taking R(T) during the cool-down does not show a sharp feature at the cubic-tetragonal transition ~100 K like the warm-up curve, presumably due to the slow kinetics of the nucleation and growth of domains, the log-log plot of temperature dependent resistance in Fig. 2a does reveal a slope change around 100 K as indicated by the black arrow and dashed line. This feature is similar to a study on the temperature dependent mobility of La-doped STO films in which a ~6 meV transverse optical soft phonon mode related to the antiferrodistortive cubic-tetragonal phase transition is invoked to explain the transport data between 10–200 K in large samples36. After patterning the sample to 40 × 40 μm2, we observed directionally dependent anisotropy in four-wire resistance at temperatures lower than ~200 K. The anisotropy also increased significantly as the temperature was lowered (Fig. 2b). It is also interesting to note the opposite trend of R(T) at T < 30 K along the two directions in Fig. 2b: while R1 shows metallic behavior (black line), R2 exhibits an upturn reminiscent of the Kondo-like scattering behavior37,38. This anisotropic behavior of R(T) along two perpendicular directions of mesoscopic device alludes to the dominance of different scattering processes. Detailed transport measurements combined with polarized light imaging on various patterned samples revealed a correlation between such electrical anisotropy in mesoscopic devices and the existence of domain wall residing within the conductive area of sample.
Reflective polarized light microscopy was used to image the conducting van der Pauw patterns post-etching. We overlaid images of domain walls with the etched patterns to obtain a clear picture how domain walls intersected the square shaped van der Pauw samples (Fig. 3a–c). By patterning the van der Pauw square parallel or at 45° angel to the ,  sides of STO substrate, we obtained three types of mesoscopic devices: (i) with no domain walls (type I, Fig. 3a), (ii) with domain walls at near 0° to the square’s edge (type II, Fig. 3b) and (iii) with domain walls 45°angle to the square’s edge (type III, Fig. 3c). In type I devices where no domain wall was residing in the device, such samples remained isotropic down to 10 K (Fig. 3d). In all type II devices, we observed at least a ten times difference between R1 and R2 at T = 10 K (Fig. 3b,e and Fig. 4), where the greater resistance (R1) is parallel to the domain wall direction. In type III devices with an extra stripped domain residing inside the pattern at ~45° angle to the measurement current direction (Fig. 3c), samples showed negligible anisotropy below 105 K (Fig. 3f), similar to the lack of anisotropy in samples with no domain walls. However, we note that Fig. 3d and f are only similar above T ~ 180 K. Below this temperature, the resistivity of the device without any domain walls (Fig. 3d) drops far more rapidly. This difference could be an interesting signature of the structural transition at ~180 K. It is also worth to point out that prior work by Schoofs et al. showed two structural transition induced hysteresis points at 85 K and 180 K35. We also clearly observed these two structural transitions in sample 10.3, whose data are displayed in Fig. 3b and e. According to our in situ polarized light imaging, the ~90 K hysteresis in R(T) is correlated with the appearance/disappearance of tetragonal domains. This leaves the exact nature of the structural phase transition at ~180 K an open question. However, since the polarized light microscopy did not detect any formation of anisotropic structures, we suspect this transition at ~180 K to be some precursor transition to the cubic-tetragonal transition at lower temperature.
The strength of anisotropic resistance is best illustrated by plotting the relative ratio between parallel and perpendicular resistances. We redefine Rparallel as the four-wire resistance measured parallel to a domain wall and Rperpendicular as the one measured perpendicular or through a domain wall. Figure 4a presents the ratio between the normalized Rparallel (T), i.e. [Rparallel(T)/Rparallel(300 K)], and the normalized Rperpendicular(T), collected on several type II devices and compare with type I devices. The tabulated values and other related sample information are listed at Table S1 in supplementary section. Upon cooling, an increasing anisotropy is observed in type II devices. In Figure 4a, one sees that the anisotropy develops as T decreases with a low T ratio in the range 10–20 in sample 10.2, 10.3 and 8.1. On the other hand, sample 10.1 showed divergent behavior in Rparallel(T) below 100 K and the anisotropy ratio reached ~105 at 10 K (Fig. 4a, inset). In type I and III devices where there are no domain walls or where the domain walls are 45° to the edges of van der Pauw square, the anisotropy remained very low (Figs 4a and S3). Changing the thickness or deposition partial pressure did not have significant effect on the anisotropy of electrical behavior as shown by comparing samples 8.1 (8 u.c. LAO, 10−5 Torr) and 10.5 (10 u.c. LAO, 10−5 Torr) to other 10 u.c. samples grown at 10−4 Torr (Fig. 4a and Table S1).
To compare the temperature scales of the increased electrical anisotropy with the structural phase transitions, we mark the positions of the ~90 K and ~180 K structural transitions as vertical dashed lines. Data in Fig. 4a show that the electrical anisotropy increases with lowering T in a smooth fashion and with no particularly sharp anomaly exhibited at ~90 K or ~180 K. However, when we compare the warm-up R(T) of micro-patterned mesoscopic devices with the R(T) during cool-down, hysteresis in R(T) is still clearly present in devices with domain walls formed inside. For instance, the structural phase transitions induced hysteresis are seen in Fig. 3e for sample 10.3. For sample 10.1 which showed the largest anisotropy at low T, hysteretic behavior is also observed in the warm-up and cool-down R(T) curves, as displayed in Fig. 4b. The persistence of hysteretic R(T) from structural phase transitions in mesoscopic devices shows that the much slower kinetics of the domain nucleation/growth during cool-down as compared to the more rapid ‘melting’ of domains upon warming up is still relevant even when individual domains with size ~10–40 μm are concerned.
Since polarized light imaging showed domain formation within those devices that exhibited anisotropy, a model explaining the electrical anisotropy should take into account the effects of domain walls on electron scattering and non-uniform carrier density/conductivity within the devices. Given the non-universal behavior of resistance anisotropy ratio vs. temperature found in different samples (Fig. 4a) and the existence of anisotropy at temperatures higher than 200 K (Figs 3e and 4a), a full account of the electrical resistance anisotropy observed here will need to take into account other temperature dependent anisotropic scattering effects that are sample specific such as anisotropic phonon scattering in the tetragonal phase, surface scattering, inhomogeneous oxygen vacancy density (e.g. random oxygen vacancy clusters) or polarization across the domain wall33,39. In particular, the surface terraces from the none zero miscut angle of STO substrate may induce a continuous temperature dependent anisotropic resistance effect throughout the whole temperature range covered here40 that interplays with the effects from structural phase transitions at ~180 K and 90 K. Note that among the four type II mesoscopic samples with ~90° domain wall in our study, sample 10.3 showed an anisotropy which continuously evolves with the temperature all the way up to 300 K (Figs 3e and 4a). Indeed, the Rparallel and Rperpendicular values for this sample differ by about seven times at 300 K (Supplementary Figure S4), the largest among all the samples. This indicates a significant pre-existing anisotropy in this sample from factors other than the structural domain effect, rationalizing the observation of an evolving anisotropy well above the structural transition temperature. Finally, it is also possible that there are additional domain structures that are not resolved by our optical microscopy34 that cause different magnitude and temperature dependence in the anisotropy found in various samples.
Motivated by the discovery of different conductivity inside a tetragonal domain vs. a domain wall as revealed in scanning SQUID (superconducting quantum interference device) and scanning electron microscopy experiments32,34, we used electromagnetic simulation software QuickField to gain some insights on the distribution of current flow and electrostatic potential in Van der Pauw square samples consisted of striped regions with different resistivity (Fig. 5). In the first case, when a striped region with lower resistivity (ρ2) representing a domain wall is sandwiched between two stripes with higher resistivity (ρ1), the same (10 nA) current through the sample induces about three times higher voltage in the configuration of current parallel to the stripe (Fig. 5b) than the perpendicular configuration (Fig. 5a), yielding Rparallel/Rperpendicular ≈ 3. On the other hand, if the triped region in the middle is set to have higher resistivity, Rparallel/Rperpendicular = 5.7 μV/34.0 μV ~ 0.167 is expected (Fig. 5c and d). This trend of having Rparallel > Rperpendicular with a lower resistivity stripe inside the sample is in qualitative agreement with prior experiments indicating domain walls having higher conductivity32,34. From the plots of current and voltage distributions in Fig. 5, one sees that the counterintuitive result of four-probe Rparallel > Rperpendicular despite domain wall being more conductive is caused by the effect of domain wall diverting current toward the voltage contacts where the resistivity is higher (Fig. 5b). If a more resistive stripe is inserted in the sample under the parallel configuration, the current flow is mostly confined within the stripe between the current contacts and thus only a weak current reaches the region between voltage contact and a small voltage is probed (Fig. 5d). This result from simulation gives a qualitative picture of why having more conductive domain walls32,34 within the van der Pauw sample can yield a higher four-probe resistance value in the parallel configuration, a somewhat counterintuitive result at first sight. Similar discussions and calculations were made in another work published recently41. However, we note that the maximum Rparallel/Rperpendicular we can induce by adjusting ρ1 and ρ2 for the simple geometry in Fig. 5 is about 3, consistent with the recent finding in ref. 41 where devices with five domains were numerically simulated. This ratio is much less than the experimental finding here of Rparallel/Rperpendicular between 10 and 105. Clearly, more complex models are needed to quantitatively account for the experimental data here. Interestingly, the experimentally measured devices containing a large number of domains in ref. 41 consistently showed a larger resistance in the current perpendicular to the domain wall configuration, in contrast to the observations for a single domain wall case in this work. This difference highlights the richness of the transport effects related to structural domains in oxide interfaces when the length scale changes.
In conclusion, we have combined the polarized light microscopy imaging of structural domains and the electrical transport to study LAO/STO devices with mesoscopic size comparable to the width of individual tetragonal domains of STO substrate. Clear temperature dependent anisotropic resistance is observed in samples split by domain walls. At low temperatures (T = 10 K), the four-point resistance is significantly lower when domain walls are perpendicular to the direction of measurement current with the anisotropy strength typically between 10–20 and sometimes reaching almost 105. These results point to the importance of considering structural inhomogeneity in understanding the complex electrical and magnetic properties of such system.
LaAlO3 (LAO) films on SrTiO3 (STO) (001) substrates with mistcut angle less than 0.5° (Crystal GmbH) were grown by Pulsed-Laser Deposition (PLD). Prior to the film growth, the SrTiO3 (STO) substrates were etched with a chemical solution of ammonium fluoride and hydrofluoric acid at pH = 6 to obtain a TiO2-terminated surface and then annealed at 950 °C for one hour in an oxygen-rich atmosphere. The surface morphology was verified with an Agilent 5500AFM. In the PLD chamber the base pressure of the chamber was 10−6 Torr and was increased to an O2 partial pressure of 10−4 Torr or 10−5 Torr via an MKS Mass Flow Controller and Cold Cathode. The growth was performed at a temperature of about 750 °C with an initial ramping rate of about 10 °C/min up to 300 °C and then about 30 °C/min up to the deposition temperature. The LAO target was ablated using a 248 nm KrF excimer laser with a fluence of about 1.2 J/cm2 and a repetition rate of 2 Hz. LAO films were grown at a rate of 9 pulses per layer and the growth rate was verified in situ by oscillations in Reflection High-Energy Electron Diffraction (RHEED) patterns. After deposition, films were cooled at an initial rate of about 10 °C/min and then a final rate of about 5 °C/min.
Mesoscopic device fabrication
Photolithography and wet etching techniques were used to reduce the sample size of LAO/STO samples (Fig. 2). Using an AutoGlow plasma system, descumming was performed in 0.6 Torr of O2 at 50 watts for 30 seconds after creating a van der Pauw pattern of photo-resist on the sample surface. Samples were then further baked at 110 °C for 20 minutes and allowed to cool slowly to reduce cracking. Wet etching was performed with buffered hydrofluoric acid for 5–7 minutes in order to etch away any LAO/STO interface not covered by the photoresist mask (Fig. 2c). After etching, the photoresist (S1805, MicroChem Inc.) was removed with acetone, revealing a clean LAO/STO van der Pauw pattern (Fig. 2d). A Zygo optical profilometer verified the etch depths were at least 6 nm. Electrical contacts were made to verify that no conductive behavior remained on etched areas. Comparing the resistance of the sample before and after the photo-lithography patterning and wet etching process shows that the device fabrication did not cause sample degradation or damage to the q2D electron system (Supplementary Fig. S5).
Structural domain imaging
Samples were placed in an RC102-CFM microscopy cryostat from Cryo Industries Inc., which were imaged using a Zeiss Axio Imager light microscope. Linear polarizer filters were used as a polarizer and analyzer for polarized transmitted light microscopy. The samples were imaged as the microscopy cryostat was cooled to 77 K using liquid nitrogen. The polarizer and analyzer filters were aligned accordingly to reveal tetragonal domain walls under 105 K. Multiple temperature cycles on many samples revealed that the domain walls do not rearrange due to thermal cycling (focusing on sample surface needs to be carefully checked between thermal cycles otherwise different domain patterns may appear due to slightly shifted focus). Electrical measurements were taken simultaneously in the microscopy cryostat using wire bonding and four-wire lock-in technique.
Samples were also measured in a QuantumDesign PPMS in of a temperature range of 10 K–300 K. Hall measurements were conducted by varying magnetic field at various temperatures. A 7 Hz sine wave was applied to the samples for electrical transport measurements. Typical current through sample was 1–100 nA. Standard four-wire lock-in techniques were used to measure the resistivity and Hall coefficients of all samples. Aluminum wire bonding was used to contact the LAO/STO interface.
How to cite this article: Goble, N. J. et al. Anisotropic electrical resistance in mesoscopic LaAlO3/SrTiO3 devices with individual domain walls. Sci. Rep. 7, 44361; doi: 10.1038/srep44361 (2017).
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Cowley, R. A. Lattice Dynamics and Phase Transitions of Strontium Titanate. Phys. Rev. 134, A981 (1964).
Lytle, F. W. X-Ray Diffractometry of Low-Temperature Phase Transformations in Strontium Titanate. J. Appl. Phys. 35, 2212 (1964).
Ohtomo, A. & Hwang, H. Y. A high-mobility electron gas at the LaAlO3/SrTiO3 heterointerface. Nature 427, 423–426 (2004).
Nakagawa, N., Hwang, H. Y. & Muller, D. A. Why some interfaces cannot be sharp. Nature Materials 5, 204–209 (2006).
Mannhart, J., Blank, D. H. A., Hwang, H. Y., Millis, A. J. & Triscone, J. M. Two-dimensional electron gases at oxide interfaces. MRS Bulletin, 33, 1027–1034 (2008).
Mannhart, J. & Schlom, D. G. Oxide Interfaces-An Opportunity for Electronics. Science 327, 1607–1611 (2010).
Hwang, H. Y., Iwasa, Y., Kawasaki, M., Keimer, B., Nagaosa, N. & Tokura, Y. Emergent phenomena at oxide interfaces. Nature Materials 11, 103–113 (2012).
Cen, C., Thiel, S., Mannhart, J. & Levy, J. Oxide nanoelectronics on demand. Science 323, 1026–1030 (2009).
Irvin, P. et al. Rewritable nanoscale oxide photodetector. Nature Photonics 4, 849–852 (2010).
Hosoda, M., Hikita, Y., Hwang, H. Y. & Bell, C. Transistor operation and mobility enhancement in top-gated LaAlO3/SrTiO3 heterostructures. Appl. Phys. Lett. 103, 103507 (2013).
Lu, H. L. et al. Reversible insulator-metal transition of LaAlO3/SrTiO3interface for nonvolatile memory. Scientific Reports 3, 2870 (2013).
Caviglia, A. D. et al. Electric field control of the LaAlO3/SrTiO3 interface ground state. Nature 456, 624–627 (2008).
Thiel, S., Hammerl, G., Schmehl, A., Schneider, C. W. & Mannhart, J. Tunable quasi-two-dimensional electron gases in oxide heterostructures. Science 313, 1942–1945 (2006).
Reyren, N. et al. Superconducting interfaces between insulating oxides. Science 317, 1196–1199 (2007).
Brinkman, A. et al. Magentic effects at the interface between non-magnetic oxides. Nature Materials 6, 493–496 (2007).
Bert, J. A. et al. Direct imaging of the coexistence of ferromagnetism and superconductivity at the LaAlO3/SrTiO3 interface. Nature Phys. 7, 767–771 (2011).
Ariando et al., Electronic phase separation at the LaAlO3/SrTiO3interface. Nature Comm. 2, 188 (2011).
Li, L., Richter, C., Mannhart, J. & Ashoori, R. C. Coexistence of magentic order and two-dimensional superconductivity at LaAlO3/SrTiO3 interfaces. Nature Phys. 7, 762–766 (2011).
Dikin, D. A. et al. Coexistence of Superconductivity and Ferromagnetism in Two Dimensions. Phys. Rev. Lett. 107, 056802 (2011).
Ramirez, A. P. Oxide electronics emerge. Science 315, 1377–1378 (2007).
Chen, Y. Z. et al. A high-mobility two-dimensional electron gas at the spinel/perovskite interface of gamma-Al2O3/SrTiO3 . Nat. Commun. 4, 1371 (2013).
Ngo, T. Q. et al. Quasi-two-dimensional electron gas at the interface of gamma-Al2O3/SrTiO3 heterostructures grown by atomic layer deposition. J. Appl. Phys. 118, 115303 (2015).
Hu, C. et al., Voltage-controlled ferromagnetism and magnetoresistance in LaCoO3/SrTiO3 heterostructures. J. Appl. Phys. 114, 183909 (2013).
Zhang, J. Y., Hwang, J., Raghavan, S. & Stemmer, S. Symmetry lowering in extreme-electron-density perovskite quantum wells, Phys. Rev. Lett. 110, 256401 (2013).
Raghavan, S., Zhang, J. Y. & Stemmer, S. Two-dimensional electron liquid at the (111) SmTiO3/SrTiO3 interface. Appl. Phys. Lett. 106, 132104 (2015).
Siemons, W. et al. Origin of charge density at LaAlO3 on SrTiO3 heterointerfaces: Possibility of intrinsic doping. Phys. Rev. Lett. 98, 196802 (2007).
Herranz, G. et al. High mobility in LaAlO3/SrTiO3 heterostructures: Origin, dimensionality, and perspectives. Phys. Rev. Lett. 98, 216803 (2007).
Kormondy, K. J. et al. Quasi-two-dimensional electron gas at the epitaxial alumina/SrTiO3 interface: Control of oxygen vacancies. Jour. Appl. Phys. 117, 095303 (2015).
Warusawithana, M. P. et al. LaAlO3 stoichiometry is key to electron liquid formation at LaAlO3/SrTiO3 interfaces. Nat. Commun. 4, 2351 (2013).
Chambers, S. A. et al. Instability, intermixing and electronic structure at the epitaxial LaAlO3/SrTiO3(001) heterojunction. Surf. Sci. Rep. 65, 317–352 (2010).
Zaid, H. et al. Atomic-resolved depth profile of strain and cation intermixing around LaAlO3/SrTiO3 interfaces. Scientific Reports 6, 28118 (2016).
Kalisky, B. et al. Locally enhanced conductivity due to the tetragonal domain structure in LaAlO3/SrTiO3 heterointerfaces. Nature Materials 12, 1091–1095 (2013).
Honig, M., Sulpizio, J. A., Drori, J., Joshua, A., Zeldov, E. & Ilani, S. Local electrostatic imaging of striped domainorder in LaAlO3/SrTiO3 . Nature Materials 12, 1112–1118 (2013).
Ma, H. J. H. et al. Local Electrical Imaging of Tetragonal Domains and Field-Induced Ferroelectric Twin Walls in Conducting SrTiO3 . Phys. Rev. Lett. 116, 257601 (2016).
Schoofs, F., Egilmez, M., Fix, T., MacManus-Driscoll, J. L. & Blamire, M. G. Impact of structural transitions on electron transport at LaAlO3/SrTiO3heterointerfaces. Appl. Phys. Lett. 100, 081601 (2012).
Verma, A., Kajdos, A. P., Cain, T. A., Stemmer, S. & Jena, D. Intrinsic mobility limiting mechanisms in lanthanum-doped strontium titanate. Phys. Rev. Lett. 112, 216601 (2014).
Lee, M., Williams, J. R., Zhang, S., Frisbie, C. D. & Goldhaber-Gordon, D., Electrolyte gate-controlled Kondo effect in SrTiO3, Phys. Rev. Lett. 107, 256601 (2011).
Han, K. et al. Controlling Kondo-like scattering at the SrTiO3-based interfaces. Sci. Rep. 6, 25455 (2016).
Zubko, P., Catalan, G., Buckley, A., Welche, P. R. L. & Scott, J. F. Strain-gradient-induced polarization in SrTiO3 single crystals. Phys Rev Lett 99, 167601 (2007).
Brinks, P., Siemons, W., Kleibeuker, J. E., Koster, G., Rijnders, G. & Huijben, M. Anisotropic electrical transport properties of a two-dimensional electron gas at SrTiO3-LaAlO3 interafaces. Appl. Phys. Lett. 98, 242904 (2011).
Frenkel, Y. et al. Anisotropic transport at the LaAlO3/SrTiO3 interface explained by microscopic imaging of channel-flow over SrTiO3 domains. ACS Appl. Mater. Interfaces 8, 12514–12519 (2016).
This work is supported by Air Force Office of Scientific Research (AFOSR) Grant FA 9550-12-1-0441. The authors thank Richard L.J. Qiu for developing the basic device fabrication and electrical characterization techniques at the early stage of the project and Walter Lambrecht for useful discussions.
The authors declare no competing financial interests.
About this article
Cite this article
Goble, N., Akrobetu, R., Zaid, H. et al. Anisotropic electrical resistance in mesoscopic LaAlO3/SrTiO3 devices with individual domain walls. Sci Rep 7, 44361 (2017). https://doi.org/10.1038/srep44361
Influence of the vicinal substrate miscut on the anisotropic two-dimensional electronic transport in Al2O3–SrTiO3 heterostructures
Journal of Applied Physics (2020)
Simple analytical method for determining electrical resistivity and sheet resistance using the van der Pauw procedure
Scientific Reports (2020)
The Journal of Physical Chemistry C (2020)
Inhomogeneous superconductivity and quasilinear magnetoresistance at amorphous LaTiO3/SrTiO3 interfaces
Journal of Physics: Condensed Matter (2020)